Water Repellent Treatment: Realiable Protection Against MoistureBy Wacker Chemie AG Editors note: The paper was presented at the seminar on Deterioration and Damaging of Mineral-Based Structures and Building - The Contemporary Protection Solution held on November 16, 2006 and is produced courtesy of IEFI Sdn Bhd.The term water-repellent treatment refers to the treatment of mineral substrates, especially facades of fair-faced masonry and concrete, with hydrophobic impregnating agents. The term impregnating agent is frequently used on its own in this context, since it is considered self- evident that these agents are hydrophobic, that is, water-repellent. By definition, however, to impregnate just means to saturate an absorbent material with a low-viscosity, capillary-active liquid.
t follows that impregnations also of masonry do not necessarily imply waterrepellent treatment. They may ser ve, for example, to strengthen and consolidate the masonry, or to imbue it with biocidal properties. In this article, however, impregnating agents are understood to be hydrophobic agents, that is, compounds which confer water repellency on mineral substrates. The purpose of water repellent treatment is to protect exposed facades from moisture and attendant damage by applying a colourless, nonfilm
forming agent which prevents capillary uptake of water and the aggressive substances dissolved therein. Because
the impregnating agent does not block the capillaries, the substrate retains its vapour permeability.
MOISTURE: ABSORPTION BY MASONRY AND RESULTING DAMAGEThe mechanisms of water uptake by building materials are as varied as the possible forms of damage to the building. This chapter deals with the mechanisms of capillary water uptake, condensation, and hygroscopic water uptake, as well as the consequences for t he building fabric.
hen mineral building materials come into contact with water, they absorb an amount which depends on their porosity. The result is various forms of damage, including: Penetration of moisture through the wall Cracks caused by swelling and shrinkage
Damage caused by frost and de icing salt Destruction of concrete caused by corrosion of the reinforcing steel Efflorescence and salt damage caused by hydration and crystallization Lime leaching Rust stains and curtaining Dirt pick up and curtaining Attack
by fungi, moss, lichens and algae Chemical corrosion, e. g. binder transformation caused by acidic gases (SO2, NO2 ) Impaired thermal insulation
831st Quarter 2007
Many of these forms of damage can be prevented, or at least reduced or kept at bay for longer, by means of impregnation. Creation of a water repellent zone considerably reduces the uptake of water and aggressive substances; the masonry remains dryer, and is consequently less prone to the kinds of damage referred to above. However, this is only true of capillary water uptake, which is the "natural" water uptake by building materials when they come into contact with water when a facade is exposed to rain, for example. There are various mechanisms of water absorption other than capillary water uptake, and
water and other liquids in the building material to a degree dependent on their capillarity. Building materials with a high proportion of such pores are generally well suited for impregnation with water repellents. these include condensation, capillary condensation, and hygroscopic water uptake. Capillary Water Uptake Capillary water uptake is responsible for the penetration of large volumes of water into the building material within a short time. The amount of water absorbed depends primarily on the radius of the capillary pores in the building material. There are three pore categories: Micropores have a radius of less than 10 7 m, gel pores less than 10 8 m. These small pores do not permit capillary water transport. Water can only penetrate these pore spaces in the form of vapou r. Consequently, building materials in which micropores dominate are practically impervious to water penetration by capillary action. They are likewise difficult to impregnate, since the water repellents cannot penetrate into these pores, either. Pores with a radius of between 107 m and 104 m are referred to as macropores or capillary pores. These pores support capillary action, and are able to transport841st Quarter 2007
Air pores, as the third pore category, have a radius exceeding 10 4 m. These large pores, like micropores, are unsuitable for capillary water transport. Capillary water absorption by mineral building materials is usually according to the squarerootoftime law. If water absorption W is plotted against the square root of the time t, a straight line is obtained, at least for the initial phase of capillary absorption. The gradient is referred to as the water absorption coefficient, or often just as the w value: Strictly speaking, the water absorption coefficient w describes the rate of capillar y absorption characteristic of a particular building material, but it is frequently used as a measure of the capillary absorbency of building materials in general. The water absorption coefficient is determined as per ISO 52617. Fig. 1 shows characteristic water absorption curves for different building materials. The w values range from 0.15 kg/m2h 0.5 for the very dense bridge concrete to 11.5 kg/m2h0.5 for the highly absorbent brick.
Stone fabric damaged by the effects of salt and moisture.
Algal growth on exposed construction elements with a high moisture content.
Hygroscopic Water Absorption The presence of soluble salts increases the equilibrium moisture content of building materials due to the salts
hygroscopicity, i.e. their ability to attract water vapour. The extent of this hygroscopic moisture absorption is determine d primarily by the chemical nature of the salts, by their
concentration in the masonry, and by the moisture content of the ambient air. Hygroscopic water absorption is especially serious when nitrates are present in the masonry.
WATER REPELLENTS: A SURE GUARANTEE OF A COMFORTABLE AMBIENCEUnlike the various film-forming coatings, building materials that have been treated with a water repellent retain their vapour permeability. This is because organosilicon water repellents do not seal the pores at the surface of the mineral masonry substrate, but form a very thin layer on the pore walls. Siliconized pores are no longer wetted by water, and capillary water uptake is prevented.be determined quantitatively as the contact angle . Untreated surfaces of mineral building materials are wetted immediately by water, i. e. the drops of water spread out and are rapidly absorbed by the building material (Fig. 3a). If the same building material is treated with an impregnating agent, the drops of water are repelled in the form of beads and do not penetrate into the substrate (Fig. 3b). Water Vapour Can Diffuse A mineral surface with (a) a hydrophobic impregnation, (b) filled pores, and (c) a sealant film. Since the pores in hydrophobically treated masonry remain open, the building material retains its vapour permeabilit y, or breathabilit y. Accordingly, the passage of water vapour is impaired only slightly, if at all. This is of great importance, since moisture contained in the building material can diffuse to the outside in the form of water vapour without causing any damage, e.g. blistering and subsequent spalling, which frequently occur with thick surface coatings.
t may be concluded from the above comments about the various water uptake mechanisms that provided the building material has pores which do permit capillary action, or the salt content at least in the surface zone is not excessively high, capillary moisture absorption without doubt poses the most serious problem. In this case, waterrepellent treatment is certainly one of the best ways to protect the masonry from moisture damage. Water repellents need to fulfill the following requirements: Drastic reduction in water uptake Retention of high watervapour permeability Extensive penetration Adequate resistance to alkalis Resistance to UV light Surfaces not rendered shiny or tacky, or caused to yellow Environmental compatibility Unlike filmforming coatings, such as those based on acrylic, polyurethane or epoxy resins, organosilicon water repellents do not seal the pores at the surface of mineral masonry, but simply form a very thin layer on the pore walls (Fig. 2). Water can no longer penetrate in liquid form into capillaries that have been
rendered waterrepellent, since, as a polar liquid, it is unable to interact with a nonpolar, hydrophobic surface. In other words, pores which have been siliconized and are therefore hydrophobic can no longer be wetted by water. The degree of wetting can
Wetting of a hydrophilic porous surface
Wetting of a hydrophobic porous surface
851st Quarter 2007
Water under Pressure is a Problem Ground water can be a serious problem in cellars, as can driving rain for highly exposed facades. The larger the pores in the building material are, the greater the problem. Since the pores are open, a waterrepellent treatment obviously cannot always protect a building material from ground water or driving
rain. However, properly applied water repellents are perfectly sufficient to render many standard building materials, such as sandlime brick, clinker brick and plasters, resistant even to driving rain with velocities of 100 km/h and more. Properly applied in this context means, for example, that the water repellent produces a hydrophobic zone which is not merely
superficial but extends to a good depth. The water repellent must accordingly be for